A comparison of Properties of laboratory prepared Cold Mixed Emulsified and Hot MixedAsphalt Mixtures
Jack N Dybalski, Manager Asphalt Technology, Akzo Chemicals Inc., McCook Illinois
Presented at the 10th Annual Meeting of the Asphalt Emulsion Manufacturers AssociationMarch 22-25 1983 Palm Springs California
Abridgement of report prepared for Akzo Chemicals Inc. by Western Technologies Inc PhoenixAZ, December 1982
TABLE OF CONTENTS
1.0 Summary . . .
4.0 Specimen Preparation
5.0 Data Matrix
6.0 Tests and Measurements
7.0 Effect of Binder Type
6.0 Effect of Gradation
9.0 Effect of Anti-Strip Treatment
10.0 Effect of Compaction Method
11.0 Effect of Cure Method
12.0 Conclusions and Recommendations
13.0 Addendum : Cure Method Variations
Asphalt emulsion cold mixes for construction of base and surface courses of bituminouspavements have been used in the United States since the 1930~s. These mixes were primarilyused on lightly traveled roads with very little, if any, documentation of their physical propertieseither before or after construction. In addition, until recently very little effort was made todevelop a generally acceptable laboratory design method for asphalt emulsion cold mixes. Amethod which engineers could use as a tool for comparison to other asphalt paving materials andmethods for pavement thickness determinations5
During the past ten years Armak Company has expended a considerable amount ofinvestigative and developmental effort toward determining those factors which are mostimportant in developing an acceptable laboratory design method for asphalt emulsion cold mixesand those factors which are necessary to obtain layer equivalency to hot mix. Concurrently,asphalt emulsion formulations of the cationic type that would adequately mix with almost anytype of aggregate without the benefit of the lubricating effect of solvent, were developed and arestill being refined5 These formulations, which solely rely upon the inherent properties of theemulsifier and the proper use of water, are essential for preparing cold mixes that adequatelycompare to the pavement-thickness criteria of hot mix.
Simply stated, in the field, asphalt emulsion layer equivalency to hot mix can be attainedby: (1) having field paving crews learn the proper use and handling of water and solvent-freecationic asphalt emulsions, (2) the use of an asphalt cement in the cold mix which is similar inviscosity or stiffness to the asphalt cement recovered from the hot mix, and (3) allowing the coldmix to cure to near its optimum stability, keeping all other variables equal.
Developing an acceptable laboratory design method for cold mixes, which reflects theirpotential equivalency to hot mix in the field, has been considerably more difficult.
Armak has, thus far, sponsored two studies at an independent testing laboratory todetermine those factors which most significantly effect the mix design criteria and resilientmoduli of asphalt emulsion cold mix compared to hot mix using two different laboratory ofspecimen preparation and evaluation -- Marshall ASTM, D-1559 and Kneading CompactionASTM, D-1561 with the Hveem Method ASTM, D-1560.
Phase I of this investigation was reported at the AEMA Annual meeting, March 17-18,1982, Las Vegas, Nevada.
The premise of this initial investigation was to emulsify an asphalt cement that hasviscosity (stiffness) properties similar to the asphalt extracted from a hot mix after the hot mixinghad been completed and to use the emulsion in the preparation of cold mixes for comparison tothe original hot mix. This was done to determine whether a cold mix versus a hot mix, bothcontaining asphalt cement of similar stiffness or viscosity, would indicate similar pavementthickness requirements.
The cold mix formula used 2% pre-wet water basis dry weight of aggregate and four setsof three specimens each at 4.0, 4.5, 5.0 and 6.0 residual asphalt respectively. A CSS-1. asphaltemulsion which contained no volatile hydrocarbon was used for the cold mix. The.hot mixspecimens were also prepared at the same asphalt content for direct comparison.
The Marshall Method of lab specimen compaction and testing was used to obtain specimendensity and stabilities. With the development of the densitylair voids data, it became evident thatMarshall Compaction, as detailed in ASTM D-1559, is not the best tab method of compaction forthese cold mix specimens. Densities and air voids equivalent to that of the hot mix wasimpossible to obtain with the Marshall Compaction Hammer, particularly with the denseaggregate.
The major problem with specimen compaction for cold mixes using the Marshall Methodis that it was designed for hot mix which contains only trace volatiles at compactiontemperatures. The mold assembly is non-porous and the tamping foot of the compaction hammeris essentially the same diameter as the inside diameter of the mold. Although 50 to 75 blows ofthe Compaction Hammer are specified for each flat side of the specimen, the water containingcold mixes often attain maxi(num attainable density after only 20 blows with rapidly developinghydraulic pore pressure causing the hammer to bounce for the remaining blows and generatingan accumulation of emulsified asphalt on the flat surfaces of the specimen.
Some work has been done with the Marshall Compaction of specimens in porous molds.However this approach has not been found to be entirely adequate because of insuffieientreduction of pore pressure under the tamping foot of the Marshall Hammer and the tendency ofsome aggregate projections to become wedged in the holes causing specimen tearing whenremoved from the mold.
Suprisingly the Resilient Modulus (Mr) (elastic Modulus) data is considerably higher for theemulsion mixes than for the hot mixes. Resilient Modulus (ElasticModuli) values have manymeanings to design engineers; however, if only these numbers were used to determine pavementthickness design, they would imply that the hot mix should be placed thicker than the cold mixfor equivalent load bearing.
This study - Phase II - used the same aggregates, Arizona Types IIIb and IVb, and thesame asphalts and AR-8000 for the cold mix and an AR-4000 for the hot mix which, whenextracted from the hot mix, has essentially the same penetration and viscosity (stiffness) as theAR-8000. Phase II, however, investigated the compaction characteristics of KneadingCompaction and the Hveem stability procedure in contrast to the Marshall method reported inPhase I. Phase II also reports the results of accelerated laboratory specimen cure in an effort toobtain density and voids values similar to the high density and low voids obtainable from coldmix placed in the field.
Kneading compaction appears to produce specimens of higher density and lower voidsthan does the Marshall. However, both methods are inadequate, as written, to obtain the densityand voids values which are comparable to the high density and low voids which are possiblefrom a 3" to 4" mat of cold mix placed in the field.
These data indicate that an appropriate laboratory specimen cure method is more importantthan the method of compaction. This will be the subject of Phase I[I.
The most important need the asphalt emulsion industry currently faces, with respect to coldmix base and surface courses, is the need for well documented and thoroughly tested fieldinstallations where data on density, voids and the development of specification stability withtime can be acquired and disseminated. These data and only these data will validate thedevelopment of a laboratory design method and acceptable design criteria.
This is a summary of a study conducted for Armak by Western Technologies, ~nc. ofPhoenix, Arizona that is a continuation of previous work that showed cold mixed pavingmixtures can be substituted on a 1 to 1 thickness basis for conventional hot mixed asphaltconcrete.
This work is intended to show the effects of aggregate gradation, compaction method,curing method, and anti-strip treatments on laboratory properties of mixtures usi~g emulsifiedasphalt and asphalt cement binders. Properties measured include:
2.1 Aggregates were crushed river gravel from Salt River siliceous deposits in Phoenix,Arizona. Gradations were dense and open conforming to The Asphalt Institute Types IV-b andIll-b as shown on Figure 1.
2.2 Asphalt cement binder was a California AR-4000. emulsified asphalt binders wereformulated solvent-free from a California AR-8000 base stock to approach CSS-1 and CMS-2properties. Anti-strip agent, when used, was Armak Redicote 82-S.
2.3 Binder contents were 4.7 and 4.9 percent by weight of mixture for open and densegradations
3.1 Asphalt cement mixtures were compacted at 230F (110C) by kneading compactor(25 tamps at 250 psi followed by 150 tamps at 500 psi).
3.2 emulsified asphalt mixtures were aerated to optimum compaction fluids content thenreceived 25 tamps of a kneading compactor at 250 psi followed by static doubleplunger loading to 40,000 pounds (177.9 kN). Following compaction, specimenswere cured in the mold for 18 hours at room temperature. After removal from molds,specimens were subjected to 12-15 in Hg (40.5 - 50.6 kPa) vacuum dessication toconstant weight. Other curing methods will be discussed later in this report.
4.0 Data matrix
4.1 Variables considered in the study are shown on Figure 2. Data were analyzed byconventional analysis of variance.
5.0 Tests and Measurements
5.1 The following tests were